Chapter 15:Characteristics, Applications & Processing of Polymers ISSUES TO ADDRESS... • What are the tensile properties of polymers and how are they affected by basic microstructural features? • Hardening, anisotropy, and annealing in polymers. • How does the elevated temperature mechanical response of polymers compare to ceramics and metals? • What are the primary polymer processing methods?
Mechanical Properties • i.e. stress-strain behavior of polymers brittle polymer FS of polymer ca. 10% that of metals plastic elastomer elastic modulus – less than metal Adapted from Fig. 15.1, Callister 7e. Strains – deformations > 1000% possible (for metals, maximum strainca. 10% or less)
fibrillar structure Near Failure near failure Initial aligned, networked crystalline cross- case regions linked slide case semi- amorphous crystalline crystalline regions case regions align elongate Tensile Response: Brittle & Plastic s (MPa) brittle failure x onset of necking plastic failure x unload/reload e Stress-strain curves adapted from Fig. 15.1, Callister 7e. Inset figures along plastic response curve adapted from Figs. 15.12 & 15.13, Callister 7e. (Figs. 15.12 & 15.13 are from J.M. Schultz, Polymer Materials Science, Prentice-Hall, Inc., 1974, pp. 500-501.)
Predeformation by Drawing • Drawing…(ex: monofilament fishline) -- stretches the polymer prior to use -- aligns chains in the stretching direction • Results of drawing: -- increases the elastic modulus (E) in the stretching direction -- increases the tensile strength (TS) in the stretching direction -- decreases ductility (%EL) • Annealing after drawing... -- decreases alignment -- reverses effects of drawing. • Compare to cold working in metals! Adapted from Fig. 15.13, Callister 7e. (Fig. 15.13 is from J.M. Schultz, Polymer Materials Science, Prentice-Hall, Inc., 1974, pp. 500-501.)
Tensile Response: Elastomer Case final: chains are straight, still cross-linked Deformation initial: amorphous chains are is reversible! kinked, cross-linked. s (MPa) brittle failure x Stress-strain curves adapted from Fig. 15.1, Callister 7e. Inset figures along elastomer curve (green) adapted from Fig. 15.15, Callister 7e. (Fig. 15.15 is from Z.D. Jastrzebski, The Nature and Properties of Engineering Materials, 3rd ed., John Wiley and Sons, 1987.) plastic failure x x elastomer e • Compare to responses of other polymers: -- brittle response (aligned, crosslinked & networked polymer) -- plastic response (semi-crystalline polymers)
Thermoplastics vs. Thermosets T Callister, rubber viscous Fig. 16.9 mobile Tm liquid tough liquid plastic Tg partially crystalline crystalline solid solid Molecular weight • Thermoplastics: -- little crosslinking -- ductile -- soften w/heating -- polyethylene polypropylene polycarbonate polystyrene • Thermosets: -- large crosslinking (10 to 50% of mers) -- hard and brittle -- do NOT soften w/heating -- vulcanized rubber, epoxies, polyester resin, phenolic resin Adapted from Fig. 15.19, Callister 7e. (Fig. 15.19 is from F.W. Billmeyer, Jr., Textbook of Polymer Science, 3rd ed., John Wiley and Sons, Inc., 1984.)
T and Strain Rate: Thermoplastics 8 0 6 0 4 0 20 s (MPa) • Decreasing T... -- increases E -- increases TS -- decreases %EL • Increasing strain rate... -- same effects as decreasing T. Data for the 4°C semicrystalline polymer: PMMA 20°C (Plexiglas) 40°C to 1.3 60°C 0 e 0 0.1 0.2 0.3 Adapted from Fig. 15.3, Callister 7e. (Fig. 15.3 is from T.S. Carswell and J.K. Nason, 'Effect of Environmental Conditions on the Mechanical Properties of Organic Plastics", Symposium on Plastics, American Society for Testing and Materials, Philadelphia, PA, 1944.)
Melting vs. Glass Transition Temp. What factors affect Tm and Tg? • Both Tm and Tg increase with increasing chain stiffness • Chain stiffness increased by • Bulky sidegroups • Polar groups or sidegroups • Double bonds or aromatic chain groups • Regularity – effects Tm only Adapted from Fig. 15.18, Callister 7e.
Time Dependent Deformation • Data: Large drop in Er for T > Tg. (amorphous polystyrene) 5 10 rigid solid Er(10s) (small relax) Adapted from Fig. 15.7, Callister 7e. (Fig. 15.7 is from A.V. Tobolsky, Properties and Structures of Polymers, John Wiley and Sons, Inc., 1960.) 3 10 in MPa transition tensile test 1 10 region eo strain -1 10 viscous liquid -3 s(t) (large relax) 10 60 100 140 180 T(°C) time Tg • Sample Tg(C) values: • Relaxation modulus: PE (low density) PE (high density) PVC PS PC -110 - 90 + 87 +100 +150 Selected values from Table 15.2, Callister 7e. • Stress relaxation test: -- strain to eo and hold. -- observe decrease in stress with time.
alligned chains microvoids fibrillar bridges crack Polymer Fracture Crazing Griffith cracks in metals – spherulites plastically deform to fibrillar structure – microvoids and fibrillar bridges form Adapted from Fig. 15.9, Callister 7e.
Propagation • Termination Addition (Chain) Polymerization • Initiation
Polymer Additives Improve mechanical properties, processability, durability, etc. • Fillers • Added to improve tensile strength & abrasion resistance, toughness & decrease cost • ex: carbon black, silica gel, wood flour, glass, limestone, talc, etc. • Plasticizers • Added to reduce the glass transition • temperature Tg • commonly added to PVC - otherwise it is brittle
Polymer Additives • Stabilizers • Antioxidants • UV protectants • Lubricants • Added to allow easier processing • “slides” through dies easier – ex: Na stearate • Colorants • Dyes or pigments • Flame Retardants • Cl/F & B
Processing of Plastics • Thermoplastic – • can be reversibly cooled & reheated, i.e. recycled • heat till soft, shape as desired, then cool • ex: polyethylene, polypropylene, polystyrene, etc. • Thermoset • when heated forms a network • degrades (not melts) when heated • mold the prepolymer then allow further reaction • ex: urethane, epoxy
Processing Plastics - Molding • Compression and transfer molding • thermoplastic or thermoset Adapted from Fig. 15.23, Callister 7e. (Fig. 15.23 is from F.W. Billmeyer, Jr., Textbook of Polymer Science, 3rd ed., John Wiley & Sons, 1984. )
Processing Plastics - Molding • Injection molding • thermoplastic & some thermosets Adapted from Fig. 15.24, Callister 7e. (Fig. 15.24 is from F.W. Billmeyer, Jr., Textbook of Polymer Science, 2nd edition, John Wiley & Sons, 1971. )
Processing Plastics – Extrusion Adapted from Fig. 15.25, Callister 7e. (Fig. 15.25 is from Encyclopædia Britannica, 1997.)
Polymer Types: Elastomers Elastomers – rubber • Crosslinked materials • Natural rubber • Synthetic rubber and thermoplastic elastomers • SBR- styrene-butadiene rubber styrene butadiene – Silicone rubber
Polymer Types: Fibers Fibers - length/diameter >100 • Textiles are main use • Must have high tensile strength • Usually highly crystalline & highly polar • Formed by spinning • ex: extrude polymer through a spinnerette • Pt plate with 1000’s of holes for nylon • ex: rayon – dissolved in solvent then pumped through die head to make fibers • the fibers are drawn • leads to highly aligned chains- fibrillar structure
Polymer Types • Coatings – thin film on surface – i.e. paint, varnish • To protect item • Improve appearance • Electrical insulation • Adhesives – produce bond between two adherands • Usually bonded by: • Secondary bonds • Mechanical bonding • Films – blown film extrusion • Foams – gas bubbles in plastic
Blown-Film Extrusion Adapted from Fig. 15.26, Callister 7e. (Fig. 15.26 is from Encyclopædia Britannica, 1997.)
Advanced Polymers • Ultrahigh molecular weight polyethylene (UHMWPE) • Molecular weight ca. 4x106 g/mol • Excellent properties for variety of applications • bullet-proof vest, golf ball covers, hip joints, etc. UHMWPE Adapted from chapter-opening photograph, Chapter 22, Callister 7e.
Summary • General drawbacks to polymers: -- E, sy, Kc, Tapplication are generally small. -- Deformation is often T and time dependent. -- Result: polymers benefit from composite reinforcement. • Thermoplastics (PE, PS, PP, PC): -- Smaller E, sy, Tapplication -- Larger Kc -- Easier to form and recycle • Elastomers (rubber): -- Large reversible strains! • Thermosets (epoxies, polyesters): -- Larger E, sy, Tapplication -- Smaller Kc Table 15.3 Callister 7e: Good overview of applications and trade names of polymers.
ANNOUNCEMENTS Reading: Core Problems: Self-help Problems: